*Corresponding author: firstname.lastname@example.org
‡both authors contributed equally to this work
Felipe Orozco1‡, Brian Alfaro-González1‡, Yendry Corrales Ureña1, Karolina Villalobos1, Angie Sanchez1, Francisco Bravo1, José Roberto Vega1 and Orlando Argüello-Miranda1†*
1National Laboratory of Nanotechnology, National Center of High Technology CENAT, San José, Costa Rica †Present address: University of Texas Southwestern Medical Center, Dallas, Texas, USA
Received November 25, 2016; Accepted January 23, 2017
ABSTRACT: As an outcome of millions of years of evolution, biological systems have developed different methods to interact with their surroundings. Many of these adaptations, such as secretions, light-interacting surfaces, biochemical active compounds, and many other survival strategies, are phenomena occurring at the nanometric scale. In this review, we describe how extracellular nanometric structures are responsible for manipulating energy and matter, creating some of the emergent properties of life. Iridescent colors in birds’ feathers, the manipulation of wettability of insects’ exoskeletons, the adhesive properties of nanopatterned secretions and the ability to polarize light are examples of the potential of extracellular nanostructures. We defined the study of extracellular nanostructures as “nanobiodiversity,” a unifying concept that emphasizes the inspiration that life at the nanoscale offers, not only for designing new materials, but also for its
KEYWORDS: Extracellular structures, biomimetic, biodiversity, nanopatterns, nanobiodiversity, evolutionary biology and bio-nanotechnology
Life on earth encompasses not only an astounding number of genetic and biochemical pathways, but also a plethora of emergent structures at the nanomet-ric scale . Nanostructures are ubiquitous through-out the phyla and achieve a variety of functions that support the survival of the species. Conservatively assuming a figure of 8 million extant species on our planet , each one producing at least one type of extracellular nanostructure, then it is likely that the most varied forms of naturally occurring nanostruc-tures are of biological origin. Precisely speaking, the replication and perpetuation of cells depends on sev-eral intracellular nanometric structures (INS), which are in charge of moving chromosomes, shaping the cell membrane, producing energy and replicating
The vision of the cell as an intricate micrometric semi-closed system run by nanometric entities, which are faithfully duplicated and passed down generation after generation, is relatively new . However, an understanding of nanometric phenomena is increas-ingly important in biology in order to explain some of the emergent properties observed in living systems. For instance, centrioles measure 250 nm in diameter and approximately 500 nm long in vertebrate cells. These nanomachines are self-assembling microtubule nucleating centers that duplicate every cell division. The mechanism of duplication of this nanomachine is still not well understood, but it involves the older copy of the centrosome functioning as a template for the new one, a property actively sought in other fields of nanotechnology . The study of INS such as cen-trioles was greatly advanced during the 20th century by the development of visualization techniques such as electron and fluorescent microscopy, as well as new methods to obtain the structure of nanometric com-plexes of proteins with RNA, DNA, and other biomol-ecules .
By contrast, the study of ENS has lagged behind probably because in many cases they are nonessential for individual cells and their biochemical passivity offered few insights into the more dynamic intracel-lular environment. The ENS were in many cases an occasional subject in tissue biology, taxonomy and, more recently, biomimetics and biomaterials . Nanopatterns on biological surfaces were mainly explored by biologists in the search for structural dif-ferences that could help to classify species .
This has led to a situation in which we have a com-mon set of general biochemical principles for intra-cellular processes, but we still do not understand the principles that rule the capacity to produce extracellu-lar nanostructures in faithful patterns . We can look into the DNA sequence of a cell and predict very pre-cisely which proteins can be synthesized, but we cannot predict very well what kind of ENS can be generated from a given genome. Furthermore, our knowledge on the diversity of naturally occurring ENS is reduced to those observed during studies with model organ-isms  or those found responsible for some beauti-ful macroscopic features, such as the structural color in hummingbirds’ feathers. Only recently have several authors approached the study of ENS from a different perspective in which evolutionary biology attempts to explain how ENS emerge in some taxa [12, 13].
Because of these reasons, we would like to argue that this emerging field of research can be described as “nanobiodiversity”: the study of extracellular nano-structures. How are ENS formed? How have they evolved? Are they directly encoded in the genome or are they the result of some cellular emergent prop-erty? What kind of mathematical or developmental principles explain the origin of ENS? These are some questions that can be addressed by investigating the nanobiodiversity of our world. This review is not intended to be exhaustive. We intend to provide sim-ple and brief examsim-ples of the most investigated extra-cellular nanostructures using original images of Costa Rican biodiversity. At the end, we provide a general description of the questions that arise when these phe-nomena are observed under the unifying concept of nanobiodiversity.
3 STRUCTURAL COLOR
Structural color in living beings is usually caused by arrays of nanometric structures that manipulate light. In many species such nano-arrangements allow for the diffraction, dispersion, absorption and/or reflection of electromagnetic radiation, which in turn produces specific colors and hues [13–18]. A great variety of liv-ing organisms have developed structural coloration: birds , reptiles , fishes , butterflies , bee-tles  and even plants .
The phenomenon is easily recognizable in irides-cent surfaces, in which the colors displayed depend on the angle of observation, sometimes granting a metal-lic appearance. Non-iridescent colors, also caused by nanostructures, do not depend on the observation angle and commonly produce bluish hues, which are rarely caused by pigmentation .
Living beings have accomplished structural col-oration by many different mechanisms. Available biomaterials are employed to develop these sophisti-cated nanostructures. Here, we describe the function of structural coloration in some species of birds and insects.
3.1 Birds (Aves)
Few colors are as impressive as a hummingbird’s iridescent feather barbules “shinning” at their best angle. Figure 1 shows the structures responsible for the copper-like coloration of the hummingbird, Elvira
cupreiceps. The mechanism consists of a b-keratin
from the one that would be shown by the melanin pig-ment alone . This is only one of the 19 mechanisms reported for avian feather barbules .
Feather barbs also present nanometric structures. That’s the case of the quasi-ordered array of mot-mot, Eumomota superciliosa, shown in Figure 1. This non-iridescent spongy medullary keratin coherently scatters light because of the size and the unimodal, but not ordered, spacing between the rods . As coloration, structural colors play a role in avian court-ship. Camouflage has also driven structural coloration to produce hues very similar to the surroundings, such as structural white plumages that mimic fallen snow .
3.2 Butterflies (Lepidoptera)
Astonishing structural colors can be found in butter-flies. They are used as warning signs between species or for mating purposes . Consistently, butterflies have developed plenty of structural color mecha-nisms. Almost one new mechanism is discovered per year .
“Lepidoptera” derives from the Greek word meaning “scale wings.” As the name suggests,
lepidopterans have micrometric chitin scales on their wings capable of manipulating light. For instance, green scales of Urania fulgens have an internal arrangement of laminar nanostructures in which air cavities are present in an organized pattern (Figure 2) . Other leptidopterans, like morpho butterflies, are famous due to their bright blue colored wings, which are a result of nanostructural arrangements on the scales, resembling closely packed Christmas trees [9, 21, 28].
3.3 Beetles (Coleoptera)
The diverse group of Coleoptera shows a large variety of species as well as a broad range of iridescent mech-anisms , which not only have cryptic and apose-matic functions  but are also for visual recognition during mating .
Three different types of iridescent mechanisms have been reported in beetles that explain how struc-tural colors operate in this clade. The first mechanism known as “multilayer reflectors” consists of nano-metric lamellae, or layers, in the endocuticle that present different refractive indexes. This has been strongly favored by the “armoured” body present in Coleoptera, in which multiple layers of cuticle provide an exoskeleton that is thicker than that of most other insects . The second mechanism is the use of three-dimensional photonic crystals, especially on scales and lattices present in several beetles such as weevils (Curculionidae) and cerambicyds (Cerambicidae). In these species, scales and lattices work as photonic devices that generate vivid colors such as the blue col-oration on Hoplia coerulea  or the green iridescence
of Lamprocyphus augustus . Finally, diffraction
gratings correspond to the third mechanism, which consists of any nanoscale array of parallel ridges or slits that disperses white light into its constituent wavelengths ; the structural color of Pallodes sp. originates from diffraction gratings.
Figure 1 Light microscope photographs of (a) Elvira cupreiceps feather barbules and (b) Eumomota superciliosa
feather barbs. Scanning electron microscopy images of the colored sections of the feathers of (c) E. cupreiceps and (d) E. superciliosa.
Figure 2 Light microscope photographs of (a) Urania fulgens
3.4 Bees, Wasps and Ants (Hymenoptera)Orchid bees (Euglossa) are widely distributed in the Neotropics and are well known for their metallic blue or green color . It has been reported that these insects reflect UV light and emit fluorescence, possibly related to the trichromatic vision of bees . On the other hand, it could also be associated with a warning mechanism for predators capable of seeing in the UV range .
The wasp Megascolia procer javanensis, for example, takes advantage of photonic nanocrystals and com-plex ENS to produce structural color. The presence of a nanostructured polymeric layer covering the wings produces an iridescent coloration, a result of the light interference patterns created by the polymer . Likewise, the surface of the bee Xylocupa viola-cea showed three layers covered with nanostructures when analyzed by AFM .
Interestingly, other ENS present in the compound eyes of some insects grant antireflective properties and enhance light transmission . Such properties have been attributed to nanostructures present on the cor-nea of butterflies and the wings of hawkmoths. In the case of compound eyes, the formation of “corneal nip-ples,” consisting of cylindrical nodules with rounded tips in a hexagonal arrangement, play a fundamen-tal role in the antireflective properties of the optical system . Similar ENS can be found in orchid bees, albeit of a more irregular morphology (Figure 3b).
Superhydrophobicity in living systems is mainly defined by nanopatterned surfaces. When a superhy-drophobic surface enters in contact with water, the complex nanometric architecture provides air pock-ets underneath the liquid droplpock-ets, promoting high contact angles (~150°) between the droplet, the solid surface and the surrounding gas . Such surfaces are present in plants like the lotus flower, the float-ing fern, roses, as well as in some insects and spiders,
which show interesting wetting properties that are being applied in biomimetic paintings and other materials .
5.1 Water Fern (Salviniaceae)
The water fern Salvinia presents an overall hydropho-bic surface due to the presence of ENS in the form of wax crystals. Additionally, hydrophilic patches cover the specialized plant trichomes (Figure 4a). This cre-ates a double-layered surface: a hydrophilic region at the top of trichomes and the hydrophobic leaf surface. Such configuration increases the energy required for water to wet the whole structure . In this manner, the leaf surface becomes superhydrophobic, and a sta-ble air layer is formed under the hydrophilic region when the fern is underwater .
5.2 Arum (Araceae)
Superhydrophibicity has also been observed in plants from the Araceae family. Different species show a series of micro-bumps covering the leaf surface. Closer inspection reveals the presence of nanofolds and wax platelets on top of the micro-bumps [43–45].
5.3 Red Rose (Rosaceae)
The red rose petals present superhydrophobicity paired with a high adhesive force (Figure 4d). When a droplet is deposited on top of the petal, it immedi-ately adopts a spherical shape, but stays anchored to the surface even at a 180° tilt angle. First described by Feng et al. , this “petal effect” is due to the micro-papillae on the surface, composed almost entirely by ENS in the form of ridges and superficial folds. Such an arrangement achieves low surface contact angles, due to the thin air layer between the nanostructures (Figure 4c), and a high adhesion, due to the capillary forces between the microstructures [43, 47].
nm 30 20 10 0 –10 –20 –30
6.1 Spiders (Arachnida)
Spider dragline fibers present different properties depending on the environmental humidity, as studied by AFM . For instance, “directional water recol-lection” , which results from the hierarchical fiber structure and allows collection of water from air mois-ture. Although the mechanism clearly takes advantage of the interactions between water droplets and the spi-der dragline polymers, it is still unclear how the wet-tability of this nanopatterned material emerges from the array of fibroin proteins.
6.2 Wasps, Bees and Ants (Hymenoptera)Insects living in highly humid environments devel-oped superhydrophobic and anti-fogging traits in the ocular area, so that condensation is restricted to the insect’s body . Pollinator insects such as bees, moths and dragonflies have a cuticle geometry in their ommatidia capable of self-cleaning. The presence of ENS reduces the surface contact between the contami-nating particles and the biological surface.
Using both SEM and AFM  revealed a correla-tion between the surface of the eye and the capacity of
self-cleaning. The van der Waals interactions between the surface of the eye and the contaminating particles may be limited, occurring only on top of a few pro-tuberances in the area of contact, resulting in a non-sticky state .
6.3 Cicadas (Hemiptera)
The presence of small, round ENS (Figure 5b) on the surface of the wings of different cicada species has been associated with important wetting and optical properties . Studies have found that the super-hydrophobicity of the wing surface promotes a self-cleaning effect, preventing major attachment of bacteria [52, 53].
7 OPTIMIZED NANOMECHANICAL
The high strength and elasticity of the dragline silk pro-duced by spiders is the perfect example of a strong and resistant nanomaterial. With a width of ~80 nm, the fibers consist of a matrix of protein crystals embedded in amorphous protein network . A combination
Figure 4 (a) Light microscope image of Salvinia sp. (b) Contact angle image of a drop of double distilled water on the surface of
of different nanometric arrangements (e.g., peptide sequences, protein conformations, surface topology) (Figure 6a) explains the spider silk’s mechanical and biological performance [54–56]. Studies comparing dif-ferent taxa of spiders  found that Argiopes sp. pro-duced a significantly stronger, and therefore tougher, silk than other spiders . Other studies, using AFM described the strength, extensibility, toughness, and stiffness of the dragline silk ; determining the number of individual silk fibers per strand (Figure 6b), while Becker et al.  characterized the stretching ability of a single fiber attached to the AFM tip.
8 NANODIVERSITY: A UNIFYING
CONCEPT BEYOND BIOMIMETICS
As seen in the previous examples, structural color, wettability and optimized nanomechanics are prop-erties of living systems that emerge from ENS. So far, these phenomena have been mainly studied from a utilitarian perspective, with scientists and engineers trying to reproduce the mechanisms found in nature . In this regard, biomimetics is a remarkable field of research aiming to create new technologies based on biological structures . For example,
biomimicry of spider silk is the base of hydrogels interwoven with nanofibers that present a high elastic modulus at low volume fractions . Studies [61–64] showed that the spider web can be mounted as films, capsules, nanofibers, and nanovesicles, with biomedical applications , and concluded that silk proteins can be used as nanowires or biosensors as well.
In a similar way, artificially generated natural iri-descent nanostructures are a promising photonic tech-nology . For instance, the production of devices, such as mirrors and filters from multilayer nanostruc-tures, is based on the iridescence mechanism from beetles (Coleoptera) . Furthermore, the clothing industry also benefits from new fabrics that reflect or absorb light depending on their nanostructured pat-tern, a property that can also be applied to computer chips [68, 69]. However, despite all of the applications and new technologies proposed by biomimetics, there are important questions that are outside their scope and they need to be addressed in order to understand how ENS are produced and maintained in the differ-ent taxa.
Structural color is an emergent property that has appeared in many species. At this point it is unclear whether the strategies to obtain structural coloration
0.00 nm (b)
Figure 5 (a) Photograph of Zamara smaragdina. (b) Atomic force microscopy images of the wing surface of Z. smaragdina.
(a) (b) (c)
are the result of a set of common rules established by natural selection or whether each strategy emerges independently, as a form of convergent evolution. In this case, we can only speculate when structural color first appeared on our planet and whether there are simple algorithms for the production of light-interacting nanostructures as proposed by Blagodatski et al. . It is also remarkable that in some taxa, such as coleopterans, many structurally different mechanisms are used to obtain iridescent colors. The necessary conditions to create this diver-sity of ENS in a single taxon are not known, but it will be of great importance to determine under which conditions the production of ENS can be pro-moted or repressed.
Superhydrophobic structures present an even more interesting scenario. For a long time, scientists created phylogenetic trees based upon defined macroscopic traits of species; it would be interesting to try to gen-erate an evolutionary tree based on an ENS-derived property, such as superhydrophobicity, which is widespread among many clades.
One of the major questions that remains to be answered is how genomes reliably produce ENS. It is unclear whether there is a minimal set of genes, proteins or developmental pathways essential for the production of ENS. Furthermore, the degree of variation of the nanostructures between individu-als from the same species is still an open question, as well as whether ENS are an example of somatic plasticity.
Experiments to test these ideas will require a com-bination of genetics, evolutionary biology and visu-alization techniques related to the areas of materials science and nanotechnology. In this regard, atomic force microscopy and electron microscopy can be valuable tools to screen for ENS across taxa.
All of these questions go beyond biomimetics and are at the crossroads between evolutionary biology and bio-nanotechnology. We believe that at this point the concept of nanobiodiversity is needed to precisely describe the multidisciplinary study of ENS. This approach can be extremely fruitful in biodiverse coun-tries such as Costa Rica and other tropical nations. For that matter, there is truly plenty of room at the bottom of biodiversity.
The authors would like to thank the Asociación Ornitológica de Costa Rica and Sistema Nacional de Áreas de Conservación for their collaboration in acquiring the samples and legal arrangements neces-sary for this work.
1. B. Bhushan, Biomimetics: Lessons from nature—an over-view. Philos. Trans. A Math. Phys. Eng. Sci.367, 1445–1486 (2009).
2. C. Mora, D.P. Tittensor, S. Adl, A.G.B. Simpson, and B. Worm, How many species are there on earth and in the ocean?. PLoS Biol. 9, e1001127 (2011).
3. B. Alberts, A. Johnson, J. Lewis, D. Morgan, M. Raff, K. Roberts, and P. Walter, Molecular Biology of the Cell, Garland Science, New York (2014).
4. B. Bhushan, Biomimetics Bioinspired Hierarchical-Structured Surfaces for Green Science and Technology, Springer, Germany (2012).
5. T. Nakano, T. Suda, Y. Okaie, M.J. Moore, and A.V. Vasilakos, Molecular communication among biological nanomachines: A layered architecture and research issues. IEEE T. Nanobiosci. 13(3), 169–197 (2014). 6. M. Winey and E. O’Toole, Centriole structure. Phil.
Trans. R. Soc. B. 369(1650), 1–9 (2014).
7. I.D. Campbell, The march of structural biology. Nat. Rev. Mol. Cell. Biol. 3(5), 377–381 (2002).
8. B.D. Ratner and S.J. Bryant, Biomaterials: Where we have been and where we are going. Annu. Rev. Biomed. Eng. 6, 41–75 (2004).
9. M.D. Shawkey, N.I. Morehouse, and P. Vukusic, A pro-tean palette: Colour materials and mixing in birds and butterflies. J. R. Soc. Interface. 6(Suppl 2), S221–S231 (2009).
10. C.M. Eliason, R. Maia, and M.D. Shawkey, Modular color evolution facilitated by a complex nanostructure in birds. Evolution. 69(2), 357–367 (2015).
11. M. Kryuchkov, V.L. Katanaev, G.A. Enin, A. Sergeev, A.A. Timchenko, and I.N. Serdyuk, Analysis of micro- and nano-structures of the corneal surface of Drosophila and its mutants by atomic force microscopy and optical diffraction. PLoS One. 6(7), e22237 (2011).
12. A. Blagodatski, A. Sergeev, M. Kryuchkov, Y. Lopatina, and V.L. Katanaev, Diverse set of Turing nanopatterns coat corneae across insect lineages. Proc. Natl. Acad. Sci. USA. 112(34), 10750–10755 (2015).
13. E.R. Dufresne, H. Noh, V. Saranathan, S.G.J. Mochrie, H. Cao, and R.O. Prum, Self-assembly of amorphous biophotonic nanostructures by phase separation. Soft Matter. 5, 1792–1795 (2009).
14. H.M. Fox and G. Vevers, The nature of animal colours.
Science133, 695–696 (1961).
15. R.O. Prum, Anatomy, physics, and evolution of structural colors, in Bird Coloration: Mechanisms and Measurements, G.E. Hill and K.J. McGraw (Eds.), Harvard University Press, Cambridge, MA (2006).
16. A.R. Parker, 515 million years of structural colour. J. Opt. A-Pure Appl. Opt. 2(6), R15–R28 (2000).
17. R. Riedler, C. Pesme, J. Druzik, M. Gleeson, and E. Pearlstein, A review of color-producing mechanisms in feathers and their influence on preventive conserva-tion strategies. J. Am. Inst. Conserv. 53(1), 44–65 (2014). 18. M.D. Shawkey and G.E. Hill, Carotenoids need
19. M. Spinner, A. Kovalev, S.N. Gorb, and G. Westhoff, Snake velvet black: Hierarchical micro- and nanostruc-ture enhances dark colouration in Bitis rhinoceros. Sci. Rep.3(1846), 1–8 (2013).
20. D. Gur, B.A. Palmer, B. Leshem, D. Oron, P. Fratzl, S. Weiner, and L. Addadi, The mechanism of color change in the neon tetra fish: A light-induced tunable photonic crystal array. Angew. Chem. Int. Ed. 54(42), 12426–12430 (2015).
21. R.O. Prum, T. Quinn, and R.H. Torres, Anatomically diverse butterfly scales all produce structural colours by coherent scattering. J. Exp. Biol. 209, 748–765 (2006). 22. A.E. Seago, P. Brady, J.-P. Vigneron, and T.D. Schultz,
Gold bugs and beyond: A review of iridescence and structural colour mechanisms in beetles (Coleoptera).
J. R. Soc. Interface, 6(Suppl 2), S165–S184 (2009).
23. S. Vignolinia, P.J. Rudall, A.V. Rowland, A. Reed, E. Moyroud, R.B. Faden, J.J. Baumberg, B.J. Glover, and U. Steiner, Pointillist structural color in Pollia fruit.
P. Natl. Acad. Sci. USA.109(39), 15712–15715 (2012). 24. D. Osorio and A.D. Ham, Spectral reflectance and
direc-tional properties of structural coloration in bird plum-age. J. Exp. Biol. 205(Pt 14), 2017–2027 (2002).
25. C.H. Greenewalt, W. Brandt, and D.D. Friel, Iridescent colors of hummingbird feathers. J. Opt. Soc. Am. 50, 1005–1013 (1960).
26. H. Durrer, The skin of birds: Colouration, in Biology of the Integument, J. Bereiter-Hahn, A.G. Matoltsy, and K.S. Richards (Eds.), Springer-Verlag, Berlin Heidelberg (1986).
27. A. Sweeney, C. Jiggins, and S. Johnsen, Insect commu-nication: Polarized light as a butterfly mating signal.
Nature. 423(6935), 31–32 (2003).
28. Y. Ding, S. Xu, and Z.L. Wang, Structural colors from
Morpho peleides butterfly wing scales. J. Appl. Phys.106, 074702 (2016).
29. T.D. Schultz, Tiger beetle defenses revisited: Alternative defense strategies and colorations of two neotropi-cal tiger beetles, Odontocheila nicaraguensis Bates and
Pseudoxycheila tarsalis Bates (Carabidae: Cicindelinae).
Coleopt. Bull. 55(2), 153–163 (2001).
30. M. Dacke, P. Nordström, C.H. Scholtz, and E.J. Warrant, A specialized dorsal rim area for polarized light detec-tion in the compound eye of the scarab beetle Pachysoma striatum. J. Comp. Physiol. 188(3), 211–216 (2002).
31. J.P. Vigneron, J.-F. Colomer, N. Vigneron, and V. Lousse, Natural layer-by-layer photonic structure in the squa-mae of Hoplia coerulea (Coleoptera). Phys. Rev. E. 72, 061904 (2005).
32. J.W. Galusha, L.R. Richey, J.S. Gardner, J.N. Cha, and M.H. Bartl, Discovery of a diamond-based photonic crys-tal structure in beetle scales. Phys. Rev. E.77, 050904(R) (2008).
33. A. Nemésio, Fluorescent colors in orchid bees (Hymenoptera: Apidae). Neotrop. Entomol. 34(6), 933–936 (2005).
34. K. Lunau, S. Papiorek, T. Eltz, and M. Sazima, Avoidance of achromatic colours by bees provides a pri-vate niche for hummingbirds. J. Exp. Biol. 214, 1607–1612 (2011).
35. O. Lind, M. Mitkus, P. Olsson, and A. Kelber, Ultraviolet vision in birds: The importance of transparent eye media.
Proc. Biol. Sci. 281(1774), 20132209 (2014).
36. M. Sarrazin, J.P. Vigneron, V. Welch, and M. Rassart, Nanomorphology of the blue iridescent wings of a giant tropical wasp, Megascolia procer javanensis
(Hymenoptera). Phys. Rev. E. 78, 051902 (2008).
37. T.R. Matin, M.K. Leong, B.Y. Majlisa, and I.C. Gebeshuber, Correlating nanostructures with func-tion: Structural colors on the wings of a Malaysian bee.
AIP Conf. Proc. 1284(1), 5–14 (2010).
38. T. Wang, W. Yu, C. Li, H. Zhang, Z. Xu, Z. Lu, and Q. Sun, Biomimetic compound eye with a high numeri-cal aperture and anti-reflective nanostructures on curved surfaces. Opt. Lett.37, 2397–2399 (2012).
39. H. Peisker and S.N. Gorb, Always on the bright side of life: Anti-adhesive properties of insect ommatidia grat-ing. J. Exp. Biol. 213, 3457–3462 (2010).
40. N. Cohen, A. Dotan, H. Dodiuk, and S. Kenig, Superhydrophobic coatings and their durability. Mater. Manuf. Process.31, 1143–1155 (2016).
41. S.S. Latthe, C. Terashima, K. Nakata, and A. Fujishima, Superhydrophobic surfaces developed by mimicking hierarchical surface morphology of lotus leaf. Molecules
19, 4256–4283 (2014).
42. W. Barthlott, T. Schimmel, S. Wiersch, K. Koch, M. Brede, M. Barczewski, S. Walheim, A. Weis, A. Kaltenmaier, A. Leder, and H.F. Bohn, The Salvinia paradox: Superhydrophobic surfaces with hydrophilic pins for air retention under water. Adv. Mater.22, 2325–2328 (2010). 43. B. Bhushan and Y.C. Jung, Wetting, adhesion and
fric-tion of superhydrophobic and hydrophilic leaves and fabricated micro/nanopatterned surfaces. J. Phys. Condens. Matter20, 225010 (2008).
44. K. Koch, H.F. Bohn, and W. Barthlott, Hierarchically sculptured plant surfaces and superhydrophobicity.
Langmuir 25, 14116–14120 (2009).
45. B. Mockenhaupt, H.-J. Ensikat, M. Spaeth, and W. Barthlott, Superhydrophobicity of biological and technical surfaces under moisture condensation: Stability in relation to surface structure. Langmuir 24, 13591–13597 (2008).
46. L. Feng, Y. Zhang, J. Xi, Y. Zhu, N. Wang, F. Xia, and L. Jiang, Petal effect: A superhydrophobic state with high adhesive force. Langmuir 24, 4114–4119 (2008). 47. G. Wang, Z. Guo, and W. Liu, Interfacial effects of
supe-rhydrophobic plant surfaces: A review. J. Bionic. Eng. 11, 325–345 (2014).
48. A. Schäfer, T. Vehoff, A. Glisovic´, and T. Salditt, Spider silk softening by water uptake: An AFM study. Eur. Biophys. J. 37, 197–204 (2008).
49. Y. Zheng, H. Bai, Z. Huang, X. Tian, F.-Q. Nie, Y. Zhao, J. Zhai, and L. Jiang, Directional water collection on wet-ted spider silk. Nature 463, 640–643 (2010).
50. Z. Sun, T. Liao, K. Liu, L. Jiang, J.H. Kim, and S.X. Dou, Fly-eye inspired superhydrophobic anti-fogging inor-ganic nanostructures. Small10, 3001–3006 (2014). 51. G.S. Watsona, D.W. Green, M. Sun, A. Liang, L. Xin,
for control of optics, wetting, adhesion, contamination, bacteria and eukaryotic cells. J. Nanosci. Adv. Technol. 1, 6–16 (2015).
52. J. Hasan, H.K. Webb, V.K. Truong, S. Pogodin, V.A. Baulin, G.S. Watson, J.A. Watson, R.J. Crawford, and E.P. Ivanova, Selective bactericidal activity of nano-patterned superhydrophobic cicada Psaltoda claripennis
wing surfaces. Appl. Microbiol. Biotechnol. 97, 9257–9262 (2013).
53. S. Pogodin, J. Hasan, V.A. Baulin, H.K. Webb, V.K. Truong, T.H. Phong Nguyen, V. Boshkovikj, C.J. Fluke, G.S. Watson, J.A. Watson, R.J. Crawford, and E.P. Ivanova, Biophysical model of bacterial cell interac-tions with nanopatterned cicada wing surfaces. Biophys. J. 104, 835–840 (2013).
54. D.M. Kane, N. Naidoo, and G.R. Staib, Atomic force microscopy of orb-spider-web-silks to measure surface nanostructuring and evaluate silk fibers per strand.
J. Appl. Phys. 108, 073509 (2010).
55. C.P. Brown, C. Harnagea, H.S. Gill, A.J. Price, E. Traversa, S. Licoccia, and F. Rosei, Rough fibrils pro-vide a toughening mechanism in biological fibers. ACS Nano6, 1961–1969 (2012).
56. S. Gomes, K. Numata, I.B. Leonor, J.F. Mano, R.L. Reis, and D.L. Kaplan, AFM study of morphology and mechan-ical properties of a chimeric spider silk and bone sialo-protein sialo-protein for bone regeneration. Biomacromolecules
12, 1675–1685 (2011).
57. B.O. Swanson, T.A. Blackledge, A.P. Summers, and C.Y. Hayashi, Spider dragline silk: Correlated and mosaic evolution in high-performance biological materi-als. Evolution 60, 2539–2551 (2006).
58. N. Becker, E. Oroudjev, S. Mutz, J.P. Cleveland, P.K. Hansma, C.Y. Hayashi, D.E. Makarov, and H.G. Hansma, Molecular nanosprings in spider capture-silk threads. Nat. Mater.2, 278–283 (2003).
59. K. Liu and L. Jiang, Bio-inspired design of multiscale structures for function integration. Nano Today 6, 155–175 (2011).
60. M. Sarikaya, C. Tamerler, A.K.-Y. Jen, K. Schulten, and F. Baneyx, Molecular biomimetics: Nanotechnology through biology. Nat. Mater.2, 577–585 (2003).
61. V.G. Bogush, O.S. Sokolova, L.I. Davydova, D.V. Klinov, K.V. Sidoruk, N.G. Esipova, T.V. Neretina, I.A. Orchanskyi, V.Y. Makeev, V.G. Tumanyan, K.V. Shaitan, V.G. Debabov, and M.P. Kirpichnikov, A novel model system for design of biomaterials based on recombinant analogs of spider silk proteins.
J. Neuroimmune Pharmacol.4, 17–27 (2009).
62. S.T. Krishnaji, W. Huang, O. Rabotyagova, E. Kharlampieva, I. Choi, V.V. Tsukruk, R. Naik, P. Cebe, and D.L. Kaplan, Thin film assembly of spi-der silk-like block copolymers. Langmuir 27, 1000–1008 (2011).
63. S. Rammensee, D. Huemmerich, K.D. Hermanson, T. Scheibel, and A.R. Bausch, Rheological characteriza-tion of hydrogels formed by recombinantly produced spider silk. Appl. Phys. A-Mater. 82, 261–264 (2006). 64. T. Scheibel, Protein fibers as performance proteins: New
technologies and applications. Curr. Opin. Biotechnol.16, 427–433 (2005).
65. H. Huang and X.S. Sun, Rational design of responsive self-assembling peptides from native protein sequences.
Biomacromolecules 11, 3390–3394 (2010).
66. E. Tamanis, I. Mihailova, B. Kokina, U. Valainis, V. Gerbreders, M. Balalaikins, A. Barševskis, and A. Ogurcovs, Surface structure and photonic nanoarchi-tectures in scales of weevils. Acta Biol. Univ. Daugavp. 14, 207–215 (2014).
67. O. Deparis, C. Vandenbem, M. Rassart, V.L. Welch, and J.-P. Vigneron, Color-selecting reflectors inspired from biological periodic multilayer structures. Opt. Express14, 3547–3555 (2006).
68. P. Ball, Nature’s color tricks. Sci. Am.306, 74–79 (2012). 69. M. Rassart, P. Simonis, A. Bay, O. Deparis, and J.P.
Vigneron, Scale coloration change following water absorption in the beetle Hoplia coerulea (Coleoptera).